#------------------------------------------------------------------------------
#$Date: 2016-03-22 12:13:13 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178941 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/70/4117014.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4117014
loop_
_publ_author_name
'Virginie Queneau'
'Slavi C. Sevov'
_publ_section_title
;
 Cs6Ge8Zn: A Zintl Phase with Isolated Heteroatomic Clusters of Ge8Zn
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              8109
_journal_page_last               8110
_journal_paper_doi               10.1021/ja9717121
_journal_volume                  119
_journal_year                    1997
_chemical_formula_sum            'Cs6 Ge8 Zn'
_chemical_formula_weight         1443.55
_chemical_name_systematic
;
 Cs6Ge8Zn
;
_space_group_IT_number           42
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'F 2 -2'
_symmetry_space_group_name_H-M   'F m m 2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            12
_cell_length_a                   22.090(2)
_cell_length_b                   23.421(4)
_cell_length_c                   12.467(2)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      11.199
_cell_measurement_theta_min      6.718
_cell_volume                     6450.1(16)
_computing_cell_refinement       CAD4_(Enraf-Nonius,_1977)
_computing_data_collection       CAD4_(Enraf-Nonius,_1977)
_computing_data_reduction        SDP_Package_(Enraf-Nonius,_1985)
_computing_molecular_graphics    'SHELXTL (Siemens, 1994)'
_computing_publication_material  'SHELXTL (Siemens, 1994)'
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device       Enraf_Nonius_CAD4
_diffrn_measurement_method       omega
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0858
_diffrn_reflns_av_sigmaI/netI    0.1253
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            3563
_diffrn_reflns_theta_max         24.99
_diffrn_reflns_theta_min         2.07
_diffrn_standards_decay_%        -0.9
_diffrn_standards_interval_count 200
_diffrn_standards_interval_time  120
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    22.098
_exptl_absorpt_correction_T_max  0.9991
_exptl_absorpt_correction_T_min  0.4821
_exptl_absorpt_correction_type   psi-scans
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.460
_exptl_crystal_description       plate-like
_exptl_crystal_F_000             7392
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.06
_refine_diff_density_max         2.229
_refine_diff_density_min         -2.396
_refine_diff_density_rms         0.465
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.45(12)
_refine_ls_extinction_coef       0.000006(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_all   1.143
_refine_ls_goodness_of_fit_obs   1.080
_refine_ls_matrix_type           full
_refine_ls_number_parameters     119
_refine_ls_number_reflns         2990
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.143
_refine_ls_restrained_S_obs      1.080
_refine_ls_R_factor_all          0.1524
_refine_ls_R_factor_obs          0.0795
_refine_ls_shift/esd_max         0.000
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0454P)²+1599.1935P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1995
_refine_ls_wR_factor_obs         0.1440
_reflns_number_observed          1766
_reflns_number_total             2990
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            ja9717121.cif
_cod_data_source_block           Cs6Ge8Zn
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0454P)^2^+1599.1935P] where P=(Fo^2^+2Fc^2^)/3'
was changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0454P)^2^+1599.1935P] where
P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_database_code               4117014
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x, -y, z'
'-x, y, z'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'x, -y+1/2, z+1/2'
'-x, y+1/2, z+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'x+1/2, -y, z+1/2'
'-x+1/2, y, z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
Cs1 Cs 0.0000 0.0000 0.9116(5) 0.029(2) Uani 1 d S
Cs2 Cs 0.8528(2) 0.0000 0.4691(4) 0.0275(11) Uani 1 d S
Cs3 Cs 0.0000 0.8164(2) 0.9121(4) 0.0386(12) Uani 1 d S
Cs4 Cs 0.0000 0.0000 0.2426(5) 0.033(2) Uani 1 d S
Cs5 Cs 0.8543(2) 0.18113(14) 0.4776(3) 0.0360(9) Uani 1 d .
Cs6 Cs 0.0000 0.1691(2) 0.2254(3) 0.0352(12) Uani 1 d S
Cs7 Cs 0.8138(2) 0.0000 0.8028(4) 0.0364(12) Uani 1 d S
Cs8 Cs 0.8094(2) 0.17119(15) 0.7948(3) 0.0422(9) Uani 1 d .
Zn1 Zn 0.8333(5) 0.0000 0.1178(8) 0.030(2) Uani 1 d S
Ge1 Ge 0.8323(3) 0.1801(2) 0.1142(5) 0.0374(13) Uani 1 d .
Ge2 Ge 0.8421(2) 0.0939(2) 0.2345(3) 0.0348(12) Uani 1 d .
Ge3 Ge 0.7290(2) 0.0937(3) 0.5660(4) 0.0342(12) Uani 1 d .
Ge4 Ge 0.8878(2) 0.9062(3) 0.0408(4) 0.0343(13) Uani 1 d .
Zn2 Zn 0.0000 0.0000 0.6137(9) 0.027(3) Uani 1 d S
Ge5 Ge 0.9407(2) 0.9069(2) 0.6769(3) 0.0271(11) Uani 1 d .
Ge6 Ge 0.0000 0.0937(3) 0.4937(5) 0.029(2) Uani 1 d S
Ge7 Ge 0.0000 0.8203(3) 0.6164(6) 0.030(2) Uani 1 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ge4 Cs1 Ge4 128.1(2) 2_666 1_446
Ge4 Cs1 Ge4 73.3(2) 2_666 4_646
Ge4 Cs1 Ge4 84.6(2) 1_446 4_646
Ge4 Cs1 Ge4 84.6(2) 2_666 3_466
Ge4 Cs1 Ge4 73.3(2) 1_446 3_466
Ge4 Cs1 Ge4 128.1(2) 4_646 3_466
Ge4 Cs1 Zn2 115.93(12) 2_666 .
Ge4 Cs1 Zn2 115.93(12) 1_446 .
Ge4 Cs1 Zn2 115.93(12) 4_646 .
Ge4 Cs1 Zn2 115.93(12) 3_466 .
Ge4 Cs1 Ge5 153.2(2) 2_666 1_445
Ge4 Cs1 Ge5 76.54(10) 1_446 1_445
Ge4 Cs1 Ge5 102.81(11) 4_646 1_445
Ge4 Cs1 Ge5 116.00(11) 3_466 1_445
Zn2 Cs1 Ge5 40.99(9) . 1_445
Ge4 Cs1 Ge5 116.00(11) 2_666 4_645
Ge4 Cs1 Ge5 102.81(11) 1_446 4_645
Ge4 Cs1 Ge5 76.54(10) 4_646 4_645
Ge4 Cs1 Ge5 153.2(2) 3_466 4_645
Zn2 Cs1 Ge5 40.99(9) . 4_645
Ge5 Cs1 Ge5 39.48(14) 1_445 4_645
Ge4 Cs1 Ge5 102.81(11) 2_666 3_465
Ge4 Cs1 Ge5 116.00(11) 1_446 3_465
Ge4 Cs1 Ge5 153.2(2) 4_646 3_465
Ge4 Cs1 Ge5 76.54(10) 3_466 3_465
Zn2 Cs1 Ge5 40.99(9) . 3_465
Ge5 Cs1 Ge5 68.4(2) 1_445 3_465
Ge5 Cs1 Ge5 82.0(2) 4_645 3_465
Ge4 Cs1 Ge5 76.54(10) 2_666 2_665
Ge4 Cs1 Ge5 153.2(2) 1_446 2_665
Ge4 Cs1 Ge5 116.00(11) 4_646 2_665
Ge4 Cs1 Ge5 102.81(11) 3_466 2_665
Zn2 Cs1 Ge5 40.99(9) . 2_665
Ge5 Cs1 Ge5 82.0(2) 1_445 2_665
Ge5 Cs1 Ge5 68.4(2) 4_645 2_665
Ge5 Cs1 Ge5 39.48(14) 3_465 2_665
Ge4 Cs1 Cs4 64.07(12) 2_666 1_556
Ge4 Cs1 Cs4 64.07(12) 1_446 1_556
Ge4 Cs1 Cs4 64.07(12) 4_646 1_556
Ge4 Cs1 Cs4 64.07(12) 3_466 1_556
Zn2 Cs1 Cs4 180.0 . 1_556
Ge5 Cs1 Cs4 139.01(9) 1_445 1_556
Ge5 Cs1 Cs4 139.01(9) 4_645 1_556
Ge5 Cs1 Cs4 139.01(9) 3_465 1_556
Ge5 Cs1 Cs4 139.01(9) 2_665 1_556
Ge4 Cs1 Cs3 126.60(12) 2_666 1_545
Ge4 Cs1 Cs3 53.32(10) 1_446 1_545
Ge4 Cs1 Cs3 53.32(10) 4_646 1_545
Ge4 Cs1 Cs3 126.60(12) 3_466 1_545
Zn2 Cs1 Cs3 90.07(12) . 1_545
Ge5 Cs1 Cs3 55.85(11) 1_445 1_545
Ge5 Cs1 Cs3 55.85(11) 4_645 1_545
Ge5 Cs1 Cs3 124.3(2) 3_465 1_545
Ge5 Cs1 Cs3 124.3(2) 2_665 1_545
Cs4 Cs1 Cs3 89.93(12) 1_556 1_545
Ge4 Cs1 Cs3 53.32(10) 2_666 2_565
Ge4 Cs1 Cs3 126.60(12) 1_446 2_565
Ge4 Cs1 Cs3 126.60(12) 4_646 2_565
Ge4 Cs1 Cs3 53.32(10) 3_466 2_565
Zn2 Cs1 Cs3 90.07(12) . 2_565
Ge5 Cs1 Cs3 124.3(2) 1_445 2_565
Ge5 Cs1 Cs3 124.3(2) 4_645 2_565
Ge5 Cs1 Cs3 55.85(11) 3_465 2_565
Ge5 Cs1 Cs3 55.85(11) 2_665 2_565
Cs4 Cs1 Cs3 89.93(12) 1_556 2_565
Cs3 Cs1 Cs3 179.9(2) 1_545 2_565
Ge2 Cs2 Ge2 73.7(2) 3 .
Ge2 Cs2 Ge3 81.81(13) 3 3
Ge2 Cs2 Ge3 124.5(2) . 3
Ge2 Cs2 Ge3 124.5(2) 3 .
Ge2 Cs2 Ge3 81.81(13) . .
Ge3 Cs2 Ge3 72.6(2) 3 .
Ge2 Cs2 Zn2 116.3(2) 3 1_655
Ge2 Cs2 Zn2 116.3(2) . 1_655
Ge3 Cs2 Zn2 119.2(2) 3 1_655
Ge3 Cs2 Zn2 119.2(2) . 1_655
Ge2 Cs2 Ge5 153.7(2) 3 3_565
Ge2 Cs2 Ge5 103.10(12) . 3_565
Ge3 Cs2 Ge5 118.8(2) 3 3_565
Ge3 Cs2 Ge5 79.66(11) . 3_565
Zn2 Cs2 Ge5 40.80(11) 1_655 3_565
Ge2 Cs2 Ge5 103.10(12) 3 1_545
Ge2 Cs2 Ge5 153.7(2) . 1_545
Ge3 Cs2 Ge5 79.66(11) 3 1_545
Ge3 Cs2 Ge5 118.8(2) . 1_545
Zn2 Cs2 Ge5 40.80(11) 1_655 1_545
Ge5 Cs2 Ge5 67.9(2) 3_565 1_545
Ge2 Cs2 Ge6 116.7(2) 3 1_655
Ge2 Cs2 Ge6 77.36(13) . 1_655
Ge3 Cs2 Ge6 156.1(2) 3 1_655
Ge3 Cs2 Ge6 104.72(13) . 1_655
Zn2 Cs2 Ge6 40.48(13) 1_655 1_655
Ge5 Cs2 Ge6 39.24(11) 3_565 1_655
Ge5 Cs2 Ge6 81.27(15) 1_545 1_655
Ge2 Cs2 Ge6 77.36(13) 3 2_655
Ge2 Cs2 Ge6 116.7(2) . 2_655
Ge3 Cs2 Ge6 104.72(13) 3 2_655
Ge3 Cs2 Ge6 156.1(2) . 2_655
Zn2 Cs2 Ge6 40.48(13) 1_655 2_655
Ge5 Cs2 Ge6 81.27(15) 3_565 2_655
Ge5 Cs2 Ge6 39.24(11) 1_545 2_655
Ge6 Cs2 Ge6 67.8(2) 1_655 2_655
Ge2 Cs2 Cs7 63.40(11) 3 10_654
Ge2 Cs2 Cs7 63.40(11) . 10_654
Ge3 Cs2 Cs7 61.15(12) 3 10_654
Ge3 Cs2 Cs7 61.15(12) . 10_654
Zn2 Cs2 Cs7 179.6(2) 1_655 10_654
Ge5 Cs2 Cs7 139.42(11) 3_565 10_654
Ge5 Cs2 Cs7 139.42(11) 1_545 10_654
Ge6 Cs2 Cs7 139.31(12) 1_655 10_654
Ge6 Cs2 Cs7 139.31(12) 2_655 10_654
Ge2 Cs2 Cs5 54.62(10) 3 3
Ge2 Cs2 Cs5 128.29(14) . 3
Ge3 Cs2 Cs5 53.57(11) 3 3
Ge3 Cs2 Cs5 126.1(2) . 3
Zn2 Cs2 Cs5 88.91(9) 1_655 3
Ge5 Cs2 Cs5 122.53(14) 3_565 3
Ge5 Cs2 Cs5 54.64(10) 1_545 3
Ge6 Cs2 Cs5 123.3(2) 1_655 3
Ge6 Cs2 Cs5 55.53(12) 2_655 3
Cs7 Cs2 Cs5 91.10(9) 10_654 3
Ge2 Cs2 Cs5 128.29(14) 3 .
Ge2 Cs2 Cs5 54.62(10) . .
Ge3 Cs2 Cs5 126.1(2) 3 .
Ge3 Cs2 Cs5 53.57(11) . .
Zn2 Cs2 Cs5 88.91(9) 1_655 .
Ge5 Cs2 Cs5 54.64(10) 3_565 .
Ge5 Cs2 Cs5 122.53(14) 1_545 .
Ge6 Cs2 Cs5 55.54(12) 1_655 .
Ge6 Cs2 Cs5 123.3(2) 2_655 .
Cs7 Cs2 Cs5 91.10(9) 10_654 .
Cs5 Cs2 Cs5 177.0(2) 3 .
Ge4 Cs3 Ge4 86.3(2) 4_656 1_456
Ge4 Cs3 Ge7 115.36(15) 4_656 .
Ge4 Cs3 Ge7 115.36(15) 1_456 .
Ge4 Cs3 Ge5 104.5(2) 4_656 1_455
Ge4 Cs3 Ge5 77.59(12) 1_456 1_455
Ge7 Cs3 Ge5 39.16(13) . 1_455
Ge4 Cs3 Ge5 77.59(12) 4_656 4_655
Ge4 Cs3 Ge5 104.5(2) 1_456 4_655
Ge7 Cs3 Ge5 39.16(13) . 4_655
Ge5 Cs3 Ge5 39.79(13) 1_455 4_655
Ge4 Cs3 Cs6 60.57(11) 4_656 2_566
Ge4 Cs3 Cs6 60.57(11) 1_456 2_566
Ge7 Cs3 Cs6 173.6(2) . 2_566
Ge5 Cs3 Cs6 135.4(2) 1_455 2_566
Ge5 Cs3 Cs6 135.4(2) 4_655 2_566
Ge4 Cs3 Ge7 100.3(2) 4_656 6_565
Ge4 Cs3 Ge7 100.27(15) 1_456 6_565
Ge7 Cs3 Ge7 129.9(2) . 6_565
Ge5 Cs3 Ge7 154.90(14) 1_455 6_565
Ge5 Cs3 Ge7 154.90(13) 4_655 6_565
Cs6 Cs3 Ge7 56.46(15) 2_566 6_565
Ge4 Cs3 Cs6 136.76(10) 4_656 5
Ge4 Cs3 Cs6 136.76(10) 1_456 5
Ge7 Cs3 Cs6 57.4(2) . 5
Ge5 Cs3 Cs6 91.76(13) 1_455 5
Ge5 Cs3 Cs6 91.76(13) 4_655 5
Cs6 Cs3 Cs6 128.96(14) 2_566 5
Ge7 Cs3 Cs6 72.5(2) 6_565 5
Ge4 Cs3 Cs1 54.58(12) 4_656 1_565
Ge4 Cs3 Cs1 54.58(12) 1_456 1_565
Ge7 Cs3 Cs1 88.5(2) . 1_565
Ge5 Cs3 Cs1 56.50(13) 1_455 1_565
Ge5 Cs3 Cs1 56.50(13) 4_655 1_565
Cs6 Cs3 Cs1 85.1(2) 2_566 1_565
Ge7 Cs3 Cs1 141.6(2) 6_565 1_565
Cs6 Cs3 Cs1 145.9(2) 5 1_565
Ge4 Cs3 Cs8 138.7(2) 4_656 3_465
Ge4 Cs3 Cs8 57.49(10) 1_456 3_465
Ge7 Cs3 Cs8 70.81(7) . 3_465
Ge5 Cs3 Cs8 52.70(9) 1_455 3_465
Ge5 Cs3 Cs8 92.05(11) 4_655 3_465
Cs6 Cs3 Cs8 108.68(7) 2_566 3_465
Ge7 Cs3 Cs8 104.75(8) 6_565 3_465
Cs6 Cs3 Cs8 82.59(8) 5 3_465
Cs1 Cs3 Cs8 86.25(9) 1_565 3_465
Ge4 Cs3 Cs8 57.49(10) 4_656 2_665
Ge4 Cs3 Cs8 138.7(2) 1_456 2_665
Ge7 Cs3 Cs8 70.81(7) . 2_665
Ge5 Cs3 Cs8 92.05(11) 1_455 2_665
Ge5 Cs3 Cs8 52.70(9) 4_655 2_665
Cs6 Cs3 Cs8 108.68(7) 2_566 2_665
Ge7 Cs3 Cs8 104.75(8) 6_565 2_665
Cs6 Cs3 Cs8 82.59(8) 5 2_665
Cs1 Cs3 Cs8 86.25(9) 1_565 2_665
Cs8 Cs3 Cs8 141.03(13) 3_465 2_665
Ge4 Cs3 Cs5 143.24(15) 4_656 5_455
Ge4 Cs3 Cs5 80.92(11) 1_456 5_455
Ge7 Cs3 Cs5 101.24(12) . 5_455
Ge5 Cs3 Cs5 106.10(9) 1_455 5_455
Ge5 Cs3 Cs5 138.99(12) 4_655 5_455
Cs6 Cs3 Cs5 83.25(9) 2_566 5_455
Ge7 Cs3 Cs5 49.39(7) 6_565 5_455
Cs6 Cs3 Cs5 61.78(8) 5 5_455
Cs1 Cs3 Cs5 133.67(7) 1_565 5_455
Cs8 Cs3 Cs5 56.08(7) 3_465 5_455
Cs8 Cs3 Cs5 139.84(12) 2_665 5_455
Ge6 Cs4 Ge6 70.0(2) 2 .
Ge6 Cs4 Cs6 58.07(14) 2 2
Ge6 Cs4 Cs6 128.1(2) . 2
Ge6 Cs4 Cs6 128.1(2) 2 .
Ge6 Cs4 Cs6 58.07(14) . .
Cs6 Cs4 Cs6 173.8(2) 2 .
Ge6 Cs4 Zn1 108.58(12) 2 1_455
Ge6 Cs4 Zn1 108.58(12) . 1_455
Cs6 Cs4 Zn1 88.80(5) 2 1_455
Cs6 Cs4 Zn1 88.80(5) . 1_455
Ge6 Cs4 Zn1 108.58(12) 2 2_655
Ge6 Cs4 Zn1 108.58(12) . 2_655
Cs6 Cs4 Zn1 88.80(5) 2 2_655
Cs6 Cs4 Zn1 88.80(5) . 2_655
Zn1 Cs4 Zn1 134.2(3) 1_455 2_655
Ge6 Cs4 Ge2 109.02(13) 2 4_655
Ge6 Cs4 Ge2 73.39(9) . 4_655
Cs6 Cs4 Ge2 122.06(8) 2 4_655
Cs6 Cs4 Ge2 57.76(8) . 4_655
Zn1 Cs4 Ge2 140.32(14) 1_455 4_655
Zn1 Cs4 Ge2 37.94(10) 2_655 4_655
Ge6 Cs4 Ge2 73.39(9) 2 3_455
Ge6 Cs4 Ge2 109.02(13) . 3_455
Cs6 Cs4 Ge2 57.76(8) 2 3_455
Cs6 Cs4 Ge2 122.06(8) . 3_455
Zn1 Cs4 Ge2 37.94(10) 1_455 3_455
Zn1 Cs4 Ge2 140.32(14) 2_655 3_455
Ge2 Cs4 Ge2 177.2(2) 4_655 3_455
Ge6 Cs4 Ge2 73.39(9) 2 2_655
Ge6 Cs4 Ge2 109.02(13) . 2_655
Cs6 Cs4 Ge2 57.76(8) 2 2_655
Cs6 Cs4 Ge2 122.06(8) . 2_655
Zn1 Cs4 Ge2 140.32(14) 1_455 2_655
Zn1 Cs4 Ge2 37.94(10) 2_655 2_655
Ge2 Cs4 Ge2 64.4(2) 4_655 2_655
Ge2 Cs4 Ge2 115.5(2) 3_455 2_655
Ge6 Cs4 Ge2 109.02(13) 2 1_455
Ge6 Cs4 Ge2 73.39(9) . 1_455
Cs6 Cs4 Ge2 122.06(8) 2 1_455
Cs6 Cs4 Ge2 57.76(8) . 1_455
Zn1 Cs4 Ge2 37.94(10) 1_455 1_455
Zn1 Cs4 Ge2 140.32(14) 2_655 1_455
Ge2 Cs4 Ge2 115.5(2) 4_655 1_455
Ge2 Cs4 Ge2 64.4(2) 3_455 1_455
Ge2 Cs4 Ge2 177.2(2) 2_655 1_455
Ge6 Cs4 Cs1 144.98(12) 2 1_554
Ge6 Cs4 Cs1 144.98(12) . 1_554
Cs6 Cs4 Cs1 86.91(12) 2 1_554
Cs6 Cs4 Cs1 86.91(12) . 1_554
Zn1 Cs4 Cs1 67.1(2) 1_455 1_554
Zn1 Cs4 Cs1 67.1(2) 2_655 1_554
Ge2 Cs4 Cs1 88.60(11) 4_655 1_554
Ge2 Cs4 Cs1 88.60(11) 3_455 1_554
Ge2 Cs4 Cs1 88.60(11) 2_655 1_554
Ge2 Cs4 Cs1 88.60(11) 1_455 1_554
Ge6 Cs4 Ge4 101.08(11) 2 1_445
Ge6 Cs4 Ge4 143.00(9) . 1_445
Cs6 Cs4 Ge4 55.93(10) 2 1_445
Cs6 Cs4 Ge4 119.67(14) . 1_445
Zn1 Cs4 Ge4 38.36(11) 1_455 1_445
Zn1 Cs4 Ge4 108.3(2) 2_655 1_445
Ge2 Cs4 Ge4 140.4(2) 4_655 1_445
Ge2 Cs4 Ge4 36.85(8) 3_455 1_445
Ge2 Cs4 Ge4 101.97(12) 2_655 1_445
Ge2 Cs4 Ge4 76.28(11) 1_455 1_445
Cs1 Cs4 Ge4 52.77(9) 1_554 1_445
Ge3 Cs5 Ge7 121.7(2) . 2_665
Ge3 Cs5 Ge2 83.10(13) . .
Ge7 Cs5 Ge2 116.8(2) 2_665 .
Ge3 Cs5 Ge1 104.9(2) . 7
Ge7 Cs5 Ge1 84.6(2) 2_665 7
Ge2 Cs5 Ge1 149.4(2) . 7
Ge3 Cs5 Ge5 82.91(12) . 3_565
Ge7 Cs5 Ge5 39.92(15) 2_665 3_565
Ge2 Cs5 Ge5 106.17(14) . 3_565
Ge1 Cs5 Ge5 104.17(14) 7 3_565
Ge3 Cs5 Ge6 109.0(2) . 1_655
Ge7 Cs5 Ge6 39.5(2) 2_665 1_655
Ge2 Cs5 Ge6 78.85(14) . 1_655
Ge1 Cs5 Ge6 123.8(2) 7 1_655
Ge5 Cs5 Ge6 40.67(11) 3_565 1_655
Ge3 Cs5 Cs8 59.10(11) . .
Ge7 Cs5 Cs8 75.81(13) 2_665 .
Ge2 Cs5 Cs8 138.68(14) . .
Ge1 Cs5 Cs8 64.70(12) 7 .
Ge5 Cs5 Cs8 56.70(10) 3_565 .
Ge6 Cs5 Cs8 97.07(12) 1_655 .
Ge3 Cs5 Cs2 55.63(12) . .
Ge7 Cs5 Cs2 90.6(2) 2_665 .
Ge2 Cs5 Cs2 54.65(12) . .
Ge1 Cs5 Cs2 152.65(15) 7 .
Ge5 Cs5 Cs2 58.06(11) 3_565 .
Ge6 Cs5 Cs2 58.14(14) 1_655 .
Cs8 Cs5 Cs2 88.01(11) . .
Ge3 Cs5 Cs8 116.39(13) . 7_554
Ge7 Cs5 Cs8 117.8(2) 2_665 7_554
Ge2 Cs5 Cs8 89.63(11) . 7_554
Ge1 Cs5 Cs8 60.16(12) 7 7_554
Ge5 Cs5 Cs8 156.84(13) 3_565 7_554
Ge6 Cs5 Cs8 131.29(14) 1_655 7_554
Cs8 Cs5 Cs8 120.51(10) . 7_554
Cs2 Cs5 Cs8 142.82(12) . 7_554
Ge3 Cs5 Cs8 58.98(11) . 12_654
Ge7 Cs5 Cs8 174.6(2) 2_665 12_654
Ge2 Cs5 Cs8 57.81(10) . 12_654
Ge1 Cs5 Cs8 100.49(14) 7 12_654
Ge5 Cs5 Cs8 138.82(13) 3_565 12_654
Ge6 Cs5 Cs8 135.29(14) 1_655 12_654
Cs8 Cs5 Cs8 107.89(9) . 12_654
Cs2 Cs5 Cs8 85.74(11) . 12_654
Cs8 Cs5 Cs8 64.06(10) 7_554 12_654
Ge3 Cs5 Cs6 136.38(14) . 1_655
Ge7 Cs5 Cs6 72.60(13) 2_665 1_655
Ge2 Cs5 Cs6 56.02(11) . 1_655
Ge1 Cs5 Cs6 117.99(14) 7 1_655
Ge5 Cs5 Cs6 93.67(11) 3_565 1_655
Ge6 Cs5 Cs6 53.25(12) 1_655 1_655
Cs8 Cs5 Cs6 147.69(10) . 1_655
Cs2 Cs5 Cs6 85.74(12) . 1_655
Cs8 Cs5 Cs6 81.04(9) 7_554 1_655
Cs8 Cs5 Cs6 103.21(8) 12_654 1_655
Ge3 Cs5 Cs3 169.17(13) . 5_644
Ge7 Cs5 Cs3 58.20(14) 2_665 5_644
Ge2 Cs5 Cs3 106.82(12) . 5_644
Ge1 Cs5 Cs3 64.38(13) 7 5_644
Ge5 Cs5 Cs3 98.07(11) 3_565 5_644
Ge6 Cs5 Cs3 77.79(13) 1_655 5_644
Cs8 Cs5 Cs3 112.46(10) . 5_644
Cs2 Cs5 Cs3 133.72(13) . 5_644
Cs8 Cs5 Cs3 60.50(8) 7_554 5_644
Cs8 Cs5 Cs3 122.36(10) 12_654 5_644
Cs6 Cs5 Cs3 54.43(9) 1_655 5_644
Ge6 Cs6 Ge7 138.8(2) . 5_544
Ge6 Cs6 Ge4 108.5(2) . 3_465
Ge7 Cs6 Ge4 102.4(2) 5_544 3_465
Ge6 Cs6 Ge4 108.5(2) . 2_665
Ge7 Cs6 Ge4 102.4(2) 5_544 2_665
Ge4 Cs6 Ge4 81.0(2) 3_465 2_665
Ge6 Cs6 Ge2 76.35(10) . 1_455
Ge7 Cs6 Ge2 115.54(10) 5_544 1_455
Ge4 Cs6 Ge2 39.60(9) 3_465 1_455
Ge4 Cs6 Ge2 112.9(2) 2_665 1_455
Ge6 Cs6 Ge2 76.35(10) . 4_655
Ge7 Cs6 Ge2 115.54(10) 5_544 4_655
Ge4 Cs6 Ge2 112.9(2) 3_465 4_655
Ge4 Cs6 Ge2 39.60(9) 2_665 4_655
Ge2 Cs6 Ge2 126.3(2) 1_455 4_655
Ge6 Cs6 Cs3 157.1(2) . 2_564
Ge7 Cs6 Cs3 64.0(2) 5_544 2_564
Ge4 Cs6 Cs3 55.85(10) 3_465 2_564
Ge4 Cs6 Cs3 55.85(10) 2_665 2_564
Ge2 Cs6 Cs3 93.89(10) 1_455 2_564
Ge2 Cs6 Cs3 93.89(10) 4_655 2_564
Ge6 Cs6 Ge1 109.85(11) . 1_455
Ge7 Cs6 Ge1 79.29(11) 5_544 1_455
Ge4 Cs6 Ge1 37.97(12) 3_465 1_455
Ge4 Cs6 Ge1 115.2(2) 2_665 1_455
Ge2 Cs6 Ge1 37.39(11) 1_455 1_455
Ge2 Cs6 Ge1 150.8(2) 4_655 1_455
Cs3 Cs6 Ge1 69.26(11) 2_564 1_455
Ge6 Cs6 Ge1 109.85(11) . 4_655
Ge7 Cs6 Ge1 79.29(11) 5_544 4_655
Ge4 Cs6 Ge1 115.2(2) 3_465 4_655
Ge4 Cs6 Ge1 37.97(12) 2_665 4_655
Ge2 Cs6 Ge1 150.8(2) 1_455 4_655
Ge2 Cs6 Ge1 37.39(11) 4_655 4_655
Cs3 Cs6 Ge1 69.26(11) 2_564 4_655
Ge1 Cs6 Ge1 138.3(2) 1_455 4_655
Ge6 Cs6 Cs4 59.1(2) . .
Ge7 Cs6 Cs4 162.1(2) 5_544 .
Ge4 Cs6 Cs4 64.60(13) 3_465 .
Ge4 Cs6 Cs4 64.60(13) 2_665 .
Ge2 Cs6 Cs4 63.15(10) 1_455 .
Ge2 Cs6 Cs4 63.15(10) 4_655 .
Cs3 Cs6 Cs4 98.1(2) 2_564 .
Ge1 Cs6 Cs4 94.79(11) 1_455 .
Ge1 Cs6 Cs4 94.79(11) 4_655 .
Ge6 Cs6 Cs3 83.8(2) . 5_544
Ge7 Cs6 Cs3 55.0(2) 5_544 5_544
Ge4 Cs6 Cs3 136.11(11) 3_465 5_544
Ge4 Cs6 Cs3 136.11(11) 2_665 5_544
Ge2 Cs6 Cs3 110.95(10) 1_455 5_544
Ge2 Cs6 Cs3 110.95(10) 4_655 5_544
Cs3 Cs6 Cs3 119.03(13) 2_564 5_544
Ge1 Cs6 Cs3 98.16(11) 1_455 5_544
Ge1 Cs6 Cs3 98.16(11) 4_655 5_544
Cs4 Cs6 Cs3 142.9(2) . 5_544
Ge6 Cs6 Cs5 54.02(8) . 4_655
Ge7 Cs6 Cs5 101.04(12) 5_544 4_655
Ge4 Cs6 Cs5 156.0(2) 3_465 4_655
Ge4 Cs6 Cs5 89.20(9) 2_665 4_655
Ge2 Cs6 Cs5 130.18(13) 1_455 4_655
Ge2 Cs6 Cs5 51.03(9) 4_655 4_655
Cs3 Cs6 Cs5 133.57(6) 2_564 4_655
Ge1 Cs6 Cs5 155.12(14) 1_455 4_655
Ge1 Cs6 Cs5 64.70(10) 4_655 4_655
Cs4 Cs6 Cs5 91.42(12) . 4_655
Cs3 Cs6 Cs5 63.79(7) 5_544 4_655
Ge5 Cs7 Ge5 68.3(2) 3_565 1_545
Ge5 Cs7 Zn1 108.8(2) 3_565 1_556
Ge5 Cs7 Zn1 108.8(2) 1_545 1_556
Ge5 Cs7 Zn1 110.8(2) 3_565 10_655
Ge5 Cs7 Zn1 110.8(2) 1_545 10_655
Zn1 Cs7 Zn1 131.6(2) 1_556 10_655
Ge5 Cs7 Cs8 124.6(2) 3_565 3
Ge5 Cs7 Cs8 56.40(10) 1_545 3
Zn1 Cs7 Cs8 91.56(10) 1_556 3
Zn1 Cs7 Cs8 88.05(10) 10_655 3
Ge5 Cs7 Cs8 56.39(10) 3_565 .
Ge5 Cs7 Cs8 124.6(2) 1_545 .
Zn1 Cs7 Cs8 91.56(10) 1_556 .
Zn1 Cs7 Cs8 88.05(10) 10_655 .
Cs8 Cs7 Cs8 176.0(2) 3 .
Ge5 Cs7 Ge4 72.48(11) 3_565 3_566
Ge5 Cs7 Ge4 108.0(2) 1_545 3_566
Zn1 Cs7 Ge4 39.24(12) 1_556 3_566
Zn1 Cs7 Ge4 139.08(14) 10_655 3_566
Cs8 Cs7 Ge4 124.9(2) 3 3_566
Cs8 Cs7 Ge4 58.95(11) . 3_566
Ge5 Cs7 Ge4 108.0(2) 3_565 1_546
Ge5 Cs7 Ge4 72.48(11) 1_545 1_546
Zn1 Cs7 Ge4 39.24(12) 1_556 1_546
Zn1 Cs7 Ge4 139.08(14) 10_655 1_546
Cs8 Cs7 Ge4 58.95(11) 3 1_546
Cs8 Cs7 Ge4 124.9(2) . 1_546
Ge4 Cs7 Ge4 65.9(2) 3_566 1_546
Ge5 Cs7 Ge3 101.02(11) 3_565 12_655
Ge5 Cs7 Ge3 143.0(2) 1_545 12_655
Zn1 Cs7 Ge3 38.91(12) 1_556 12_655
Zn1 Cs7 Ge3 106.2(2) 10_655 12_655
Cs8 Cs7 Ge3 123.7(2) 3 12_655
Cs8 Cs7 Ge3 58.26(11) . 12_655
Ge4 Cs7 Ge3 37.44(10) 3_566 12_655
Ge4 Cs7 Ge3 78.14(14) 1_546 12_655
Ge5 Cs7 Ge3 143.0(2) 3_565 10_655
Ge5 Cs7 Ge3 101.02(11) 1_545 10_655
Zn1 Cs7 Ge3 38.91(12) 1_556 10_655
Zn1 Cs7 Ge3 106.2(2) 10_655 10_655
Cs8 Cs7 Ge3 58.26(11) 3 10_655
Cs8 Cs7 Ge3 123.7(2) . 10_655
Ge4 Cs7 Ge3 78.14(14) 3_566 10_655
Ge4 Cs7 Ge3 37.44(10) 1_546 10_655
Ge3 Cs7 Ge3 65.5(2) 12_655 10_655
Ge5 Cs7 Ge3 74.94(11) 3_565 .
Ge5 Cs7 Ge3 109.7(2) 1_545 .
Zn1 Cs7 Ge3 139.50(14) 1_556 .
Zn1 Cs7 Ge3 38.37(11) 10_655 .
Cs8 Cs7 Ge3 120.2(2) 3 .
Cs8 Cs7 Ge3 55.94(10) . .
Ge4 Cs7 Ge3 114.83(10) 3_566 .
Ge4 Cs7 Ge3 176.9(2) 1_546 .
Ge3 Cs7 Ge3 100.67(13) 12_655 .
Ge3 Cs7 Ge3 139.48(14) 10_655 .
Ge5 Cs7 Ge3 109.7(2) 3_565 3
Ge5 Cs7 Ge3 74.94(11) 1_545 3
Zn1 Cs7 Ge3 139.50(14) 1_556 3
Zn1 Cs7 Ge3 38.37(11) 10_655 3
Cs8 Cs7 Ge3 55.94(10) 3 3
Cs8 Cs7 Ge3 120.2(2) . 3
Ge4 Cs7 Ge3 176.9(2) 3_566 3
Ge4 Cs7 Ge3 114.83(10) 1_546 3
Ge3 Cs7 Ge3 139.48(14) 12_655 3
Ge3 Cs7 Ge3 100.67(13) 10_655 3
Ge3 Cs7 Ge3 64.2(2) . 3
Ge5 Cs8 Ge3 80.46(12) 3_565 .
Ge5 Cs8 Ge1 115.26(15) 3_565 12_655
Ge3 Cs8 Ge1 38.09(12) . 12_655
Ge5 Cs8 Ge2 111.42(14) 3_565 12_655
Ge3 Cs8 Ge2 39.82(10) . 12_655
Ge1 Cs8 Ge2 38.07(12) 12_655 12_655
Ge5 Cs8 Ge3 106.27(13) 3_565 12_655
Ge3 Cs8 Ge3 108.85(15) . 12_655
Ge1 Cs8 Ge3 110.61(15) 12_655 12_655
Ge2 Cs8 Ge3 76.43(11) 12_655 12_655
Ge5 Cs8 Ge4 74.96(11) 3_565 3_566
Ge3 Cs8 Ge4 124.36(14) . 3_566
Ge1 Cs8 Ge4 146.2(2) 12_655 3_566
Ge2 Cs8 Ge4 108.31(14) 12_655 3_566
Ge3 Cs8 Ge4 38.47(10) 12_655 3_566
Ge5 Cs8 Cs7 60.07(13) 3_565 .
Ge3 Cs8 Cs7 63.57(13) . .
Ge1 Cs8 Cs7 95.04(13) 12_655 .
Ge2 Cs8 Cs7 63.82(12) 12_655 .
Ge3 Cs8 Cs7 61.47(13) 12_655 .
Ge4 Cs8 Cs7 60.86(13) 3_566 .
Ge5 Cs8 Ge1 108.52(14) 3_565 1_556
Ge3 Cs8 Ge1 145.4(2) . 1_556
Ge1 Cs8 Ge1 132.63(14) 12_655 1_556
Ge2 Cs8 Ge1 108.98(14) 12_655 1_556
Ge3 Cs8 Ge1 36.75(12) 12_655 1_556
Ge4 Cs8 Ge1 37.02(12) 3_566 1_556
Cs7 Cs8 Ge1 91.38(14) . 1_556
Ge5 Cs8 Cs5 57.14(10) 3_565 .
Ge3 Cs8 Cs5 54.32(10) . .
Ge1 Cs8 Cs5 68.23(13) 12_655 .
Ge2 Cs8 Cs5 92.77(11) 12_655 .
Ge3 Cs8 Cs5 155.76(13) 12_655 .
Ge4 Cs8 Cs5 132.01(13) 3_566 .
Cs7 Cs8 Cs5 94.30(12) . .
Ge1 Cs8 Cs5 157.77(14) 1_556 .
Ge5 Cs8 Ge1 95.85(14) 3_565 7
Ge3 Cs8 Ge1 92.87(14) . 7
Ge1 Cs8 Ge1 74.9(2) 12_655 7
Ge2 Cs8 Ge1 112.93(15) 12_655 7
Ge3 Cs8 Ge1 151.02(15) 12_655 7
Ge4 Cs8 Ge1 138.19(15) 3_566 7
Cs7 Cs8 Ge1 147.51(15) . 7
Ge1 Cs8 Ge1 118.39(12) 1_556 7
Cs5 Cs8 Ge1 53.22(10) . 7
Ge5 Cs8 Cs5 115.32(13) 3_565 7
Ge3 Cs8 Cs5 153.36(14) . 7
Ge1 Cs8 Cs5 117.21(13) 12_655 7
Ge2 Cs8 Cs5 133.17(13) 12_655 7
Ge3 Cs8 Cs5 88.00(11) 12_655 7
Ge4 Cs8 Cs5 81.69(11) 3_566 7
Cs7 Cs8 Cs5 142.45(14) . 7
Ge1 Cs8 Cs5 53.04(9) 1_556 7
Cs5 Cs8 Cs5 114.52(10) . 7
Ge1 Cs8 Cs5 65.35(10) 7 7
Ge5 Cs8 Cs5 153.28(14) 3_565 12_655
Ge3 Cs8 Cs5 91.76(11) . 12_655
Ge1 Cs8 Cs5 67.84(13) 12_655 12_655
Ge2 Cs8 Cs5 53.13(10) 12_655 12_655
Ge3 Cs8 Cs5 52.06(9) 12_655 12_655
Ge4 Cs8 Cs5 89.00(11) 3_566 12_655
Cs7 Cs8 Cs5 93.54(12) . 12_655
Ge1 Cs8 Cs5 64.94(13) 1_556 12_655
Cs5 Cs8 Cs5 135.86(10) . 12_655
Ge1 Cs8 Cs5 110.12(13) 7 12_655
Cs5 Cs8 Cs5 82.41(10) 7 12_655
Ge2 Zn1 Ge2 112.6(4) 3 .
Ge2 Zn1 Ge3 59.1(2) 3 10_654
Ge2 Zn1 Ge3 148.7(5) . 10_654
Ge2 Zn1 Ge3 148.7(5) 3 12_654
Ge2 Zn1 Ge3 59.1(2) . 12_654
Ge3 Zn1 Ge3 110.6(4) 10_654 12_654
Ge2 Zn1 Ge4 147.7(5) 3 3_565
Ge2 Zn1 Ge4 58.9(2) . 3_565
Ge3 Zn1 Ge4 144.9(4) 10_654 3_565
Ge3 Zn1 Ge4 58.1(2) 12_654 3_565
Ge2 Zn1 Ge4 58.9(2) 3 1_545
Ge2 Zn1 Ge4 147.7(5) . 1_545
Ge3 Zn1 Ge4 58.1(2) 10_654 1_545
Ge3 Zn1 Ge4 144.9(4) 12_654 1_545
Ge4 Zn1 Ge4 109.9(4) 3_565 1_545
Ge2 Zn1 Cs7 123.7(2) 3 1_554
Ge2 Zn1 Cs7 123.7(2) . 1_554
Ge3 Zn1 Cs7 72.7(2) 10_654 1_554
Ge3 Zn1 Cs7 72.7(2) 12_654 1_554
Ge4 Zn1 Cs7 72.1(2) 3_565 1_554
Ge4 Zn1 Cs7 72.1(2) 1_545 1_554
Ge2 Zn1 Cs7 75.0(2) 3 10_654
Ge2 Zn1 Cs7 75.0(2) . 10_654
Ge3 Zn1 Cs7 73.7(2) 10_654 10_654
Ge3 Zn1 Cs7 73.7(2) 12_654 10_654
Ge4 Zn1 Cs7 125.0(2) 3_565 10_654
Ge4 Zn1 Cs7 125.0(2) 1_545 10_654
Cs7 Zn1 Cs7 119.1(3) 1_554 10_654
Ge2 Zn1 Cs4 73.6(2) 3 1_655
Ge2 Zn1 Cs4 73.6(2) . 1_655
Ge3 Zn1 Cs4 124.7(2) 10_654 1_655
Ge3 Zn1 Cs4 124.7(2) 12_654 1_655
Ge4 Zn1 Cs4 74.1(2) 3_565 1_655
Ge4 Zn1 Cs4 74.1(2) 1_545 1_655
Cs7 Zn1 Cs4 119.2(3) 1_554 1_655
Cs7 Zn1 Cs4 121.7(3) 10_654 1_655
Ge2 Zn1 Cs2 56.3(2) 3 .
Ge2 Zn1 Cs2 56.3(2) . .
Ge3 Zn1 Cs2 106.9(2) 10_654 .
Ge3 Zn1 Cs2 106.9(2) 12_654 .
Ge4 Zn1 Cs2 108.2(2) 3_565 .
Ge4 Zn1 Cs2 108.2(2) 1_545 .
Cs7 Zn1 Cs2 179.3(3) 1_554 .
Cs7 Zn1 Cs2 60.2(2) 10_654 .
Cs4 Zn1 Cs2 61.5(2) 1_655 .
Ge3 Ge1 Ge2 62.8(2) 12_654 .
Ge3 Ge1 Ge4 62.1(2) 12_654 3_565
Ge2 Ge1 Ge4 62.3(2) . 3_565
Ge3 Ge1 Cs5 132.0(3) 12_654 7_554
Ge2 Ge1 Cs5 164.7(3) . 7_554
Ge4 Ge1 Cs5 118.0(3) 3_565 7_554
Ge3 Ge1 Cs8 70.1(2) 12_654 12_654
Ge2 Ge1 Cs8 71.3(2) . 12_654
Ge4 Ge1 Cs8 124.1(2) 3_565 12_654
Cs5 Ge1 Cs8 114.9(2) 7_554 12_654
Ge3 Ge1 Cs6 122.4(2) 12_654 1_655
Ge2 Ge1 Cs6 70.2(2) . 1_655
Ge4 Ge1 Cs6 67.8(2) 3_565 1_655
Cs5 Ge1 Cs6 95.5(2) 7_554 1_655
Cs8 Ge1 Cs6 123.4(2) 12_654 1_655
Ge3 Ge1 Cs8 69.7(2) 12_654 1_554
Ge2 Ge1 Cs8 123.9(2) . 1_554
Ge4 Ge1 Cs8 70.2(2) 3_565 1_554
Cs5 Ge1 Cs8 66.80(12) 7_554 1_554
Cs8 Ge1 Cs8 118.2(2) 12_654 1_554
Cs6 Ge1 Cs8 117.5(2) 1_655 1_554
Ge3 Ge1 Cs8 137.4(3) 12_654 7_554
Ge2 Ge1 Cs8 110.9(2) . 7_554
Ge4 Ge1 Cs8 156.6(3) 3_565 7_554
Cs5 Ge1 Cs8 62.08(10) 7_554 7_554
Cs8 Ge1 Cs8 68.42(14) 12_654 7_554
Cs6 Ge1 Cs8 88.8(2) 1_655 7_554
Cs8 Ge1 Cs8 124.16(15) 1_554 7_554
Ge1 Ge2 Ge4 59.0(2) . 3_565
Ge1 Ge2 Ge3 58.3(2) . 12_654
Ge4 Ge2 Ge3 59.5(2) 3_565 12_654
Ge1 Ge2 Zn1 109.4(3) . .
Ge4 Ge2 Zn1 61.3(3) 3_565 .
Ge3 Ge2 Zn1 60.9(3) 12_654 .
Ge1 Ge2 Cs5 92.9(2) . .
Ge4 Ge2 Cs5 137.3(2) 3_565 .
Ge3 Ge2 Cs5 135.0(2) 12_654 .
Zn1 Ge2 Cs5 157.5(3) . .
Ge1 Ge2 Cs2 163.5(2) . .
Ge4 Ge2 Cs2 135.3(2) 3_565 .
Ge3 Ge2 Cs2 132.6(2) 12_654 .
Zn1 Ge2 Cs2 86.9(2) . .
Cs5 Ge2 Cs2 70.73(10) . .
Ge1 Ge2 Cs8 70.6(2) . 12_654
Ge4 Ge2 Cs8 120.8(2) 3_565 12_654
Ge3 Ge2 Cs8 68.9(2) 12_654 12_654
Zn1 Ge2 Cs8 115.6(3) . 12_654
Cs5 Ge2 Cs8 69.06(12) . 12_654
Cs2 Ge2 Cs8 100.41(14) . 12_654
Ge1 Ge2 Cs6 72.5(2) . 1_655
Ge4 Ge2 Cs6 68.2(2) 3_565 1_655
Ge3 Ge2 Cs6 120.8(2) 12_654 1_655
Zn1 Ge2 Cs6 115.1(3) . 1_655
Cs5 Ge2 Cs6 72.95(13) . 1_655
Cs2 Ge2 Cs6 103.64(15) . 1_655
Cs8 Ge2 Cs6 124.4(2) 12_654 1_655
Ge1 Ge2 Cs4 120.9(2) . 1_655
Ge4 Ge2 Cs4 72.3(2) 3_565 1_655
Ge3 Ge2 Cs4 121.7(2) 12_654 1_655
Zn1 Ge2 Cs4 68.4(3) . 1_655
Cs5 Ge2 Cs4 102.40(14) . 1_655
Cs2 Ge2 Cs4 66.83(13) . 1_655
Cs8 Ge2 Cs4 166.9(2) 12_654 1_655
Cs6 Ge2 Cs4 59.09(10) 1_655 1_655
Ge1 Ge2 Cs7 118.2(2) . 10_654
Ge4 Ge2 Cs7 120.4(2) 3_565 10_654
Ge3 Ge2 Cs7 70.7(2) 12_654 10_654
Zn1 Ge2 Cs7 67.3(3) . 10_654
Cs5 Ge2 Cs7 100.70(13) . 10_654
Cs2 Ge2 Cs7 64.81(13) . 10_654
Cs8 Ge2 Cs7 59.65(9) 12_654 10_654
Cs6 Ge2 Cs7 168.4(2) 1_655 10_654
Cs4 Ge2 Cs7 114.34(14) 1_655 10_654
Ge1 Ge3 Ge4 59.5(2) 12_655 10_665
Ge1 Ge3 Ge2 58.9(2) 12_655 12_655
Ge4 Ge3 Ge2 60.2(2) 10_665 12_655
Ge1 Ge3 Zn1 109.1(2) 12_655 10_655
Ge4 Ge3 Zn1 61.2(3) 10_665 10_655
Ge2 Ge3 Zn1 59.9(2) 12_655 10_655
Ge1 Ge3 Cs5 91.7(2) 12_655 .
Ge4 Ge3 Cs5 136.3(3) 10_665 .
Ge2 Ge3 Cs5 134.6(2) 12_655 .
Zn1 Ge3 Cs5 159.1(3) 10_655 .
Ge1 Ge3 Cs2 162.5(3) 12_655 .
Ge4 Ge3 Cs2 133.9(2) 10_665 .
Ge2 Ge3 Cs2 134.7(2) 12_655 .
Zn1 Ge3 Cs2 88.4(2) 10_655 .
Cs5 Ge3 Cs2 70.80(10) . .
Ge1 Ge3 Cs8 71.9(2) 12_655 .
Ge4 Ge3 Cs8 123.5(2) 10_665 .
Ge2 Ge3 Cs8 71.3(2) 12_655 .
Zn1 Ge3 Cs8 116.7(3) 10_655 .
Cs5 Ge3 Cs8 66.58(12) . .
Cs2 Ge3 Cs8 100.46(14) . .
Ge1 Ge3 Cs8 73.6(2) 12_655 12_654
Ge4 Ge3 Cs8 71.4(2) 10_665 12_654
Ge2 Ge3 Cs8 124.0(2) 12_655 12_654
Zn1 Ge3 Cs8 118.5(3) 10_655 12_654
Cs5 Ge3 Cs8 68.97(12) . 12_654
Cs2 Ge3 Cs8 98.74(13) . 12_654
Cs8 Ge3 Cs8 121.6(2) . 12_654
Ge1 Ge3 Cs7 120.3(2) 12_655 10_654
Ge4 Ge3 Cs7 70.9(2) 10_665 10_654
Ge2 Ge3 Cs7 120.6(2) 12_655 10_654
Zn1 Ge3 Cs7 68.4(2) 10_655 10_654
Cs5 Ge3 Cs7 103.76(14) . 10_654
Cs2 Ge3 Cs7 65.68(12) . 10_654
Cs8 Ge3 Cs7 165.7(2) . 10_654
Cs8 Ge3 Cs7 60.27(10) 12_654 10_654
Ge1 Ge3 Cs7 120.2(2) 12_655 .
Ge4 Ge3 Cs7 122.5(2) 10_665 .
Ge2 Ge3 Cs7 72.5(2) 12_655 .
Zn1 Ge3 Cs7 67.9(3) 10_655 .
Cs5 Ge3 Cs7 99.88(14) . .
Cs2 Ge3 Cs7 65.40(12) . .
Cs8 Ge3 Cs7 60.49(10) . .
Cs8 Ge3 Cs7 163.5(2) 12_654 .
Cs7 Ge3 Cs7 113.34(14) 10_654 .
Ge1 Ge4 Ge3 58.4(2) 3_565 10_664
Ge1 Ge4 Ge2 58.6(2) 3_565 3_565
Ge3 Ge4 Ge2 60.3(2) 10_664 3_565
Ge1 Ge4 Zn1 107.8(2) 3_565 1_565
Ge3 Ge4 Zn1 60.7(3) 10_664 1_565
Ge2 Ge4 Zn1 59.8(2) 3_565 1_565
Ge1 Ge4 Cs3 91.6(2) 3_565 1_654
Ge3 Ge4 Cs3 137.1(3) 10_664 1_654
Ge2 Ge4 Cs3 132.2(2) 3_565 1_654
Zn1 Ge4 Cs3 160.1(3) 1_565 1_654
Ge1 Ge4 Cs1 163.6(2) 3_565 1_664
Ge3 Ge4 Cs1 136.1(2) 10_664 1_664
Ge2 Ge4 Cs1 131.5(2) 3_565 1_664
Zn1 Ge4 Cs1 88.3(2) 1_565 1_664
Cs3 Ge4 Cs1 72.10(11) 1_654 1_664
Ge1 Ge4 Cs6 74.2(2) 3_565 2_665
Ge3 Ge4 Cs6 124.9(2) 10_664 2_665
Ge2 Ge4 Cs6 72.2(2) 3_565 2_665
Zn1 Ge4 Cs6 117.0(3) 1_565 2_665
Cs3 Ge4 Cs6 63.58(12) 1_654 2_665
Cs1 Ge4 Cs6 95.89(13) 1_664 2_665
Ge1 Ge4 Cs8 72.7(2) 3_565 3_564
Ge3 Ge4 Cs8 70.1(2) 10_664 3_564
Ge2 Ge4 Cs8 123.0(2) 3_565 3_564
Zn1 Ge4 Cs8 117.1(3) 1_565 3_564
Cs3 Ge4 Cs8 72.01(13) 1_654 3_564
Cs1 Ge4 Cs8 103.24(15) 1_664 3_564
Cs6 Ge4 Cs8 122.7(2) 2_665 3_564
Ge1 Ge4 Cs7 120.2(2) 3_565 1_564
Ge3 Ge4 Cs7 71.7(2) 10_664 1_564
Ge2 Ge4 Cs7 121.4(2) 3_565 1_564
Zn1 Ge4 Cs7 68.6(2) 1_565 1_564
Cs3 Ge4 Cs7 105.51(15) 1_654 1_564
Cs1 Ge4 Cs7 68.08(13) 1_664 1_564
Cs6 Ge4 Cs7 163.4(2) 2_665 1_564
Cs8 Ge4 Cs7 60.19(10) 3_564 1_564
Ge1 Ge4 Cs4 119.4(2) 3_565 1_665
Ge3 Ge4 Cs4 121.2(2) 10_664 1_665
Ge2 Ge4 Cs4 70.9(2) 3_565 1_665
Zn1 Ge4 Cs4 67.6(2) 1_565 1_665
Cs3 Ge4 Cs4 99.62(12) 1_654 1_665
Cs1 Ge4 Cs4 63.15(14) 1_664 1_665
Cs6 Ge4 Cs4 59.47(10) 2_665 1_665
Cs8 Ge4 Cs4 166.1(2) 3_564 1_665
Cs7 Ge4 Cs4 113.5(2) 1_564 1_665
Ge6 Zn2 Ge6 111.4(5) . 2
Ge6 Zn2 Ge5 59.3(2) . 2_665
Ge6 Zn2 Ge5 147.5(3) 2 2_665
Ge6 Zn2 Ge5 147.5(3) . 1_445
Ge6 Zn2 Ge5 59.3(2) 2 1_445
Ge5 Zn2 Ge5 145.6(5) 2_665 1_445
Ge6 Zn2 Ge5 59.3(2) . 3_465
Ge6 Zn2 Ge5 147.5(3) 2 3_465
Ge5 Zn2 Ge5 58.9(2) 2_665 3_465
Ge5 Zn2 Ge5 109.9(3) 1_445 3_465
Ge6 Zn2 Ge5 147.5(3) . 4_645
Ge6 Zn2 Ge5 59.3(2) 2 4_645
Ge5 Zn2 Ge5 109.9(3) 2_665 4_645
Ge5 Zn2 Ge5 58.9(2) 1_445 4_645
Ge5 Zn2 Ge5 145.6(5) 3_465 4_645
Ge6 Zn2 Cs1 124.3(3) . .
Ge6 Zn2 Cs1 124.3(3) 2 .
Ge5 Zn2 Cs1 72.8(3) 2_665 .
Ge5 Zn2 Cs1 72.8(3) 1_445 .
Ge5 Zn2 Cs1 72.8(3) 3_465 .
Ge5 Zn2 Cs1 72.8(3) 4_645 .
Ge6 Zn2 Cs2 74.2(2) . 1_455
Ge6 Zn2 Cs2 74.2(2) 2 1_455
Ge5 Zn2 Cs2 125.01(14) 2_665 1_455
Ge5 Zn2 Cs2 73.33(13) 1_445 1_455
Ge5 Zn2 Cs2 73.33(13) 3_465 1_455
Ge5 Zn2 Cs2 125.01(14) 4_645 1_455
Cs1 Zn2 Cs2 119.0(2) . 1_455
Ge6 Zn2 Cs2 74.2(2) . 2_655
Ge6 Zn2 Cs2 74.2(2) 2 2_655
Ge5 Zn2 Cs2 73.33(13) 2_665 2_655
Ge5 Zn2 Cs2 125.01(14) 1_445 2_655
Ge5 Zn2 Cs2 125.01(14) 3_465 2_655
Ge5 Zn2 Cs2 73.33(13) 4_645 2_655
Cs1 Zn2 Cs2 119.0(2) . 2_655
Cs2 Zn2 Cs2 122.0(3) 1_455 2_655
Ge7 Ge5 Ge5 58.82(14) 1_655 4_755
Ge7 Ge5 Ge6 58.6(3) 1_655 2_665
Ge5 Ge5 Ge6 60.17(12) 4_755 2_665
Ge7 Ge5 Zn2 108.3(2) 1_655 1_665
Ge5 Ge5 Zn2 60.53(11) 4_755 1_665
Ge6 Ge5 Zn2 60.2(3) 2_665 1_665
Ge7 Ge5 Cs8 97.3(2) 1_655 3_565
Ge5 Ge5 Cs8 141.03(9) 4_755 3_565
Ge6 Ge5 Cs8 136.5(2) 2_665 3_565
Zn2 Ge5 Cs8 154.2(2) 1_665 3_565
Ge7 Ge5 Cs5 68.0(2) 1_655 3_565
Ge5 Ge5 Cs5 120.59(9) 4_755 3_565
Ge6 Ge5 Cs5 71.1(2) 2_665 3_565
Zn2 Ge5 Cs5 120.3(3) 1_665 3_565
Cs8 Ge5 Cs5 66.16(11) 3_565 3_565
Ge7 Ge5 Cs3 67.0(2) 1_655 1_655
Ge5 Ge5 Cs3 70.10(7) 4_755 1_655
Ge6 Ge5 Cs3 119.3(2) 2_665 1_655
Zn2 Ge5 Cs3 120.6(2) 1_665 1_655
Cs8 Ge5 Cs3 72.20(11) 3_565 1_655
Cs5 Ge5 Cs3 112.0(2) 3_565 1_655
Ge7 Ge5 Cs1 120.1(2) 1_655 1_665
Ge5 Ge5 Cs1 70.26(7) 4_755 1_665
Ge6 Ge5 Cs1 119.3(2) 2_665 1_665
Zn2 Ge5 Cs1 66.2(3) 1_665 1_665
Cs8 Ge5 Cs1 103.93(13) 3_565 1_665
Cs5 Ge5 Cs1 168.81(14) 3_565 1_665
Cs3 Ge5 Cs1 67.64(11) 1_655 1_665
Ge7 Ge5 Cs7 160.8(2) 1_655 1_565
Ge5 Ge5 Cs7 136.23(10) 4_755 1_565
Ge6 Ge5 Cs7 135.5(2) 2_665 1_565
Zn2 Ge5 Cs7 90.9(2) 1_665 1_565
Cs8 Ge5 Cs7 63.54(9) 3_565 1_565
Cs5 Ge5 Cs7 102.05(14) 3_565 1_565
Cs3 Ge5 Cs7 104.30(13) 1_655 1_565
Cs1 Ge5 Cs7 67.86(11) 1_665 1_565
Ge7 Ge5 Cs2 120.5(2) 1_655 1_565
Ge5 Ge5 Cs2 119.85(9) 4_755 1_565
Ge6 Ge5 Cs2 71.0(2) 2_665 1_565
Zn2 Ge5 Cs2 65.9(2) 1_665 1_565
Cs8 Ge5 Cs2 98.53(13) 3_565 1_565
Cs5 Ge5 Cs2 67.30(10) 3_565 1_565
Cs3 Ge5 Cs2 169.34(14) 1_655 1_565
Cs1 Ge5 Cs2 110.79(14) 1_665 1_565
Cs7 Ge5 Cs2 66.13(12) 1_565 1_565
Ge7 Ge6 Ge5 58.6(2) 2_565 2_665
Ge7 Ge6 Ge5 58.6(2) 2_565 3_465
Ge5 Ge6 Ge5 59.7(2) 2_665 3_465
Ge7 Ge6 Zn2 108.5(3) 2_565 .
Ge5 Ge6 Zn2 60.5(2) 2_665 .
Ge5 Ge6 Zn2 60.5(2) 3_465 .
Ge7 Ge6 Cs6 99.4(3) 2_565 .
Ge5 Ge6 Cs6 140.3(2) 2_665 .
Ge5 Ge6 Cs6 140.3(2) 3_465 .
Zn2 Ge6 Cs6 152.1(3) . .
Ge7 Ge6 Cs5 66.73(15) 2_565 4_655
Ge5 Ge6 Cs5 68.25(14) 2_665 4_655
Ge5 Ge6 Cs5 117.9(2) 3_465 4_655
Zn2 Ge6 Cs5 118.21(12) . 4_655
Cs6 Ge6 Cs5 72.73(13) . 4_655
Ge7 Ge6 Cs5 66.73(15) 2_565 1_455
Ge5 Ge6 Cs5 117.9(2) 2_665 1_455
Ge5 Ge6 Cs5 68.25(14) 3_465 1_455
Zn2 Ge6 Cs5 118.21(12) . 1_455
Cs6 Ge6 Cs5 72.73(13) . 1_455
Cs5 Ge6 Cs5 114.8(2) 4_655 1_455
Ge7 Ge6 Cs4 162.2(3) 2_565 .
Ge5 Ge6 Cs4 135.0(2) 2_665 .
Ge5 Ge6 Cs4 135.0(2) 3_465 .
Zn2 Ge6 Cs4 89.3(3) . .
Cs6 Ge6 Cs4 62.86(13) . .
Cs5 Ge6 Cs4 105.34(12) 4_655 .
Cs5 Ge6 Cs4 105.34(12) 1_455 .
Ge7 Ge6 Cs2 119.42(12) 2_565 1_455
Ge5 Ge6 Cs2 118.4(2) 2_665 1_455
Ge5 Ge6 Cs2 69.7(2) 3_465 1_455
Zn2 Ge6 Cs2 65.4(2) . 1_455
Cs6 Ge6 Cs2 101.03(12) . 1_455
Cs5 Ge6 Cs2 172.3(2) 4_655 1_455
Cs5 Ge6 Cs2 66.33(6) 1_455 1_455
Cs4 Ge6 Cs2 67.43(12) . 1_455
Ge7 Ge6 Cs2 119.42(12) 2_565 2_655
Ge5 Ge6 Cs2 69.7(2) 2_665 2_655
Ge5 Ge6 Cs2 118.4(2) 3_465 2_655
Zn2 Ge6 Cs2 65.4(2) . 2_655
Cs6 Ge6 Cs2 101.03(12) . 2_655
Cs5 Ge6 Cs2 66.33(6) 4_655 2_655
Cs5 Ge6 Cs2 172.3(2) 1_455 2_655
Cs4 Ge6 Cs2 67.43(12) . 2_655
Cs2 Ge6 Cs2 111.5(2) 1_455 2_655
Ge5 Ge7 Ge5 62.4(3) 4_655 1_455
Ge5 Ge7 Ge6 62.7(2) 4_655 2_565
Ge5 Ge7 Ge6 62.7(2) 1_455 2_565
Ge5 Ge7 Cs5 127.2(3) 4_655 3_465
Ge5 Ge7 Cs5 72.09(14) 1_455 3_465
Ge6 Ge7 Cs5 73.8(2) 2_565 3_465
Ge5 Ge7 Cs5 72.09(14) 4_655 2_665
Ge5 Ge7 Cs5 127.2(3) 1_455 2_665
Ge6 Ge7 Cs5 73.8(2) 2_565 2_665
Cs5 Ge7 Cs5 123.4(2) 3_465 2_665
Ge5 Ge7 Cs3 73.9(2) 4_655 .
Ge5 Ge7 Cs3 73.9(2) 1_455 .
Ge6 Ge7 Cs3 128.6(3) 2_565 .
Cs5 Ge7 Cs3 118.25(12) 3_465 .
Cs5 Ge7 Cs3 118.25(12) 2_665 .
Ge5 Ge7 Cs6 129.9(3) 4_655 5
Ge5 Ge7 Cs6 129.9(3) 1_455 5
Ge6 Ge7 Cs6 163.8(3) 2_565 5
Cs5 Ge7 Cs6 99.27(15) 3_465 5
Cs5 Ge7 Cs6 99.27(15) 2_665 5
Cs3 Ge7 Cs6 67.6(2) . 5
Ge5 Ge7 Cs3 144.4(2) 4_655 6_564
Ge5 Ge7 Cs3 144.4(2) 1_455 6_564
Ge6 Ge7 Cs3 104.3(3) 2_565 6_564
Cs5 Ge7 Cs3 72.41(13) 3_465 6_564
Cs5 Ge7 Cs3 72.41(13) 2_665 6_564
Cs3 Ge7 Cs3 127.1(2) . 6_564
Cs6 Ge7 Cs3 59.50(14) 5 6_564
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cs1 Ge4 3.682(6) 2_666
Cs1 Ge4 3.682(6) 1_446
Cs1 Ge4 3.682(6) 4_646
Cs1 Ge4 3.682(6) 3_466
Cs1 Zn2 3.714(14) .
Cs1 Ge5 3.877(7) 1_445
Cs1 Ge5 3.877(7) 4_645
Cs1 Ge5 3.877(7) 3_465
Cs1 Ge5 3.877(7) 2_665
Cs1 Cs4 4.126(9) 1_556
Cs1 Cs3 4.300(5) 1_545
Cs1 Cs3 4.300(5) 2_565
Cs2 Ge2 3.667(6) 3
Cs2 Ge2 3.667(6) .
Cs2 Ge3 3.709(6) 3
Cs2 Ge3 3.709(6) .
Cs2 Zn2 3.719(7) 1_655
Cs2 Ge5 3.903(6) 3_565
Cs2 Ge5 3.903(6) 1_545
Cs2 Ge6 3.935(6) 1_655
Cs2 Ge6 3.935(6) 2_655
Cs2 Cs7 4.223(7) 10_654
Cs2 Cs5 4.244(3) 3
Cs2 Cs5 4.244(3) .
Cs3 Ge4 3.624(6) 4_656
Cs3 Ge4 3.624(6) 1_456
Cs3 Ge7 3.687(10) .
Cs3 Ge5 3.848(7) 1_455
Cs3 Ge5 3.848(7) 4_655
Cs3 Cs6 3.921(6) 2_566
Cs3 Ge7 4.092(10) 6_565
Cs3 Cs6 4.161(7) 5
Cs3 Cs1 4.300(5) 1_565
Cs3 Cs8 4.467(4) 3_465
Cs3 Cs8 4.467(4) 2_665
Cs3 Cs5 4.590(5) 5_455
Cs4 Ge6 3.823(8) 2
Cs4 Ge6 3.823(8) .
Cs4 Cs6 3.966(5) 2
Cs4 Cs6 3.966(5) .
Cs4 Zn1 3.997(11) 1_455
Cs4 Zn1 3.997(11) 2_655
Cs4 Ge2 4.125(5) 4_655
Cs4 Ge2 4.125(5) 3_455
Cs4 Ge2 4.125(5) 2_655
Cs4 Ge2 4.125(5) 1_455
Cs4 Cs1 4.126(9) 1_554
Cs4 Ge4 4.159(6) 1_445
Cs5 Ge3 3.616(6) .
Cs5 Ge7 3.655(5) 2_665
Cs5 Ge2 3.666(6) .
Cs5 Ge1 3.702(6) 7
Cs5 Ge5 3.751(6) 3_565
Cs5 Ge6 3.820(6) 1_655
Cs5 Cs8 4.085(5) .
Cs5 Cs8 4.259(4) 7_554
Cs5 Cs8 4.279(5) 12_654
Cs5 Cs6 4.508(5) 1_655
Cs5 Cs3 4.590(5) 5_644
Cs6 Ge6 3.782(8) .
Cs6 Ge7 3.793(9) 5_544
Cs6 Ge4 3.814(6) 3_465
Cs6 Ge4 3.814(6) 2_665
Cs6 Ge2 3.910(6) 1_455
Cs6 Ge2 3.910(6) 4_655
Cs6 Cs3 3.922(6) 2_564
Cs6 Ge1 3.963(8) 1_455
Cs6 Ge1 3.963(8) 4_655
Cs6 Cs3 4.161(7) 5_544
Cs6 Cs5 4.508(5) 4_655
Cs7 Ge5 3.884(6) 3_565
Cs7 Ge5 3.884(6) 1_545
Cs7 Zn1 3.951(11) 1_556
Cs7 Zn1 3.984(12) 10_655
Cs7 Cs8 4.012(4) 3
Cs7 Cs8 4.012(4) .
Cs7 Ge4 4.038(7) 3_566
Cs7 Ge4 4.038(7) 1_546
Cs7 Ge3 4.059(7) 12_655
Cs7 Ge3 4.059(7) 10_655
Cs7 Ge3 4.128(7) .
Cs7 Ge3 4.128(7) 3
Cs8 Ge5 3.732(6) 3_565
Cs8 Ge3 3.819(6) .
Cs8 Ge1 3.861(8) 12_655
Cs8 Ge2 3.878(6) 12_655
Cs8 Ge3 3.929(7) 12_655
Cs8 Ge4 3.961(7) 3_566
Cs8 Ge1 4.019(7) 1_556
Cs8 Ge1 4.179(7) 7
Cs8 Cs5 4.259(4) 7
Cs8 Cs5 4.279(5) 12_655
Zn1 Ge2 2.643(8) 3
Zn1 Ge2 2.643(8) .
Zn1 Ge3 2.669(8) 10_654
Zn1 Ge3 2.669(8) 12_654
Zn1 Ge4 2.684(8) 3_565
Zn1 Ge4 2.684(8) 1_545
Zn1 Cs7 3.951(11) 1_554
Zn1 Cs7 3.984(12) 10_654
Zn1 Cs4 3.997(11) 1_655
Ge1 Ge3 2.507(8) 12_654
Ge1 Ge2 2.524(8) .
Ge1 Ge4 2.534(8) 3_565
Ge1 Cs5 3.702(6) 7_554
Ge1 Cs8 3.861(8) 12_654
Ge1 Cs6 3.963(8) 1_655
Ge1 Cs8 4.019(7) 1_554
Ge1 Cs8 4.179(7) 7_554
Ge2 Ge4 2.618(6) 3_565
Ge2 Ge3 2.622(6) 12_654
Ge2 Cs8 3.878(6) 12_654
Ge2 Cs6 3.910(6) 1_655
Ge2 Cs4 4.125(5) 1_655
Ge2 Cs7 4.172(7) 10_654
Ge3 Ge1 2.507(8) 12_655
Ge3 Ge4 2.599(7) 10_665
Ge3 Ge2 2.622(6) 12_655
Ge3 Zn1 2.669(8) 10_655
Ge3 Cs8 3.929(7) 12_654
Ge3 Cs7 4.059(7) 10_654
Ge4 Ge1 2.534(8) 3_565
Ge4 Ge3 2.599(7) 10_664
Ge4 Ge2 2.618(6) 3_565
Ge4 Zn1 2.684(8) 1_565
Ge4 Cs3 3.624(6) 1_654
Ge4 Cs1 3.682(6) 1_664
Ge4 Cs6 3.814(6) 2_665
Ge4 Cs8 3.961(7) 3_564
Ge4 Cs7 4.038(7) 1_564
Ge4 Cs4 4.159(6) 1_665
Zn2 Ge6 2.656(10) .
Zn2 Ge6 2.656(10) 2
Zn2 Ge5 2.662(6) 2_665
Zn2 Ge5 2.662(6) 1_445
Zn2 Ge5 2.662(6) 3_465
Zn2 Ge5 2.662(6) 4_645
Zn2 Cs2 3.719(7) 1_455
Zn2 Cs2 3.719(7) 2_655
Ge5 Ge7 2.530(9) 1_655
Ge5 Ge5 2.619(9) 4_755
Ge5 Ge6 2.632(6) 2_665
Ge5 Zn2 2.662(6) 1_665
Ge5 Cs8 3.732(6) 3_565
Ge5 Cs5 3.751(6) 3_565
Ge5 Cs3 3.848(7) 1_655
Ge5 Cs1 3.877(7) 1_665
Ge5 Cs7 3.884(6) 1_565
Ge5 Cs2 3.903(6) 1_565
Ge6 Ge7 2.530(11) 2_565
Ge6 Ge5 2.632(6) 2_665
Ge6 Ge5 2.632(6) 3_465
Ge6 Cs5 3.820(6) 4_655
Ge6 Cs5 3.820(6) 1_455
Ge6 Cs2 3.935(6) 1_455
Ge6 Cs2 3.935(6) 2_655
Ge7 Ge5 2.530(9) 4_655
Ge7 Ge5 2.530(9) 1_455
Ge7 Ge6 2.530(11) 2_565
Ge7 Cs5 3.655(5) 3_465
Ge7 Cs5 3.655(5) 2_665
Ge7 Cs6 3.793(9) 5
Ge7 Cs3 4.092(10) 6_564
